Recent work has proposed that enhanced efficiency can be achieved in photovoltaic cells through implementation of the intermediate band (IB) concept in which a narrow band inserted within the band gap of a semiconductor is used to make the combined absorption of two sub-band gap energy photons lead to the generation of current at the higher voltage corresponding to the full band gap. Trying to tell which materials could have the IB properties necessary for this, quantum calculations within density functional theory at the generalized gradient approximation level have been carried out in this work for chalcopyrite-type copper gallium sulphide structures where gallium is partially substituted by transition metal atoms (Ti, V, Cr, Mn), as these materials are presumed to be candidates for developing the IB electronic structure able to realize this concept. The computed electronic structures characterized by density-of-state curves and band dispersion diagrams, show transition metal-induced spin-polarized characteristics and additional bands appearing in the band gap of the parent sulphide compound. In the results reported here for these compounds, the multiplicity, degree of filling, and energy position of the electronic levels depends on the number of electrons and the electronegativity of the transition element, and they are analyzed in terms of the crystal field splitting produced by the crystalline structure in the metal $3d$ orbital manifold. For the Ti- and Cr-derived structures (the more interesting ones from the point of view of the intermediate band photovoltaic concept), the stability of these materials is also assessed by computing the energetics of their decomposition in appropriate, known stable compounds. Although this decomposition is found to be favorable, the corresponding energy difference is relatively small, and it is envisaged that they can be made effective experimentally. With these results, the suitability of these materials for use as IB compounds in photovoltaic cells is discussed, and the Ti-substituted one is proposed as the best candidate of this type.

1.
Luque
,
A.
, and
Martí
,
A.
, 1997, “
Increasing the Efficiency of Ideal Solar Cells by Photon Induced Transitions at Intermediate Levels
,”
Phys. Rev. Lett.
0031-9007,
78
(
26
), pp.
5014
5017
.
2.
Luque
,
A.
, and
Martí
,
A.
, 2001, “
A Metallic intermediate Band High Efficiency Solar Cell
,”
Prog. Photovoltaics
1062-7995,
9
(
2
), pp.
73
86
.
3.
Picozzi
,
S.
,
Zhao
,
Y. J.
,
Freeman
,
A. J.
, and
Delley
,
B.
, 2002, “
Mn-Doped CuGaS2 Chalcopyrite: An Ab Initio Study of Ferromagnetic Semiconductors
,”
Phys. Rev. B
0163-1829,
66
,
205206
.
4.
Zhao
,
Y. J.
, and
Zunger
,
A.
, 2004, “
Electronic Structure and Ferromagnetism of Mn-substituted CuAlS2, CuGaS2, CuInS2, CuGaSe2, CuGaTe2
,”
Phys. Rev. B
0163-1829,
69
,
104422
.
5.
Wahnón
,
P.
, and
Tablero
,
C.
, 2002, “
Ab Initio Electronic Structure Calculations for Metallic Intermediate Band Formation in Photovoltaic Materials
,”
Phys. Rev. B
0163-1829,
65
(
16
)
165115
;
Wahnón
,
P.
,
Palacios
,
P.
,
Fernández
,
J. J.
, and
Tablero
,
C.
, 2005, “
Ab-Initio Spin Polarized Electronic Structure Calculations for TixGanAsm Photovoltaic Materials
,”
J. Mater. Sci.
0022-2461,
40
(
6
), pp.
1383
1386
.
6.
Perdew
,
J. P.
, and
Wang
,
Y.
, 1992, “
Accurate and Simple Analytic Representation of the Electron-Gas Correlation-Energy
,”
Phys. Rev. B
0163-1829,
45
(
23
), pp.
13244
13249
.
7.
Kresse
,
G.
, and
Hafner
,
J.
, 1993, “
Abinitio Molecular-Dynamics for Liquid-Metals
,”
Phys. Rev. B
0163-1829,
47
(
1
), pp.
558
561
;
Kresse
,
G.
, and
Furthmüller
,
J.
, 1996, “
Efficient Iterative Schemes for Ab Initio Total-Energy Calculations using a Plane-Wave Basis Set
,”
Phys. Rev. B
0163-1829,
54
(
16
), pp.
11169
11186
.
8.
Monkhorst
,
H. J.
, and
Pack
,
J. D.
, 1977, “
Special Points for Brillouin-Zone Integrations—A Reply
,”
Phys. Rev. B
0556-2805,
16
(
4
), pp.
1748
1749
.
9.
Palacios
,
P.
,
Fernández
,
J. J.
,
Sánchez
,
K.
,
Conesa
,
J. C.
, and
Wahnón
,
P.
, 2006, “
First Principles Investigation of Isolated Band Formation in Half-Metallic TixGa1−xP (x=0.3125–0.25)
,”
Phys. Rev. B
0163-1829,
73
,
085206
.
10.
Shirakata
,
S.
,
Murakami
,
K.
, and
Kukimoto
,
H.
, 1989, “
Electroreflectance Studies in CuGaS2
,”
Jpn. J. Appl. Phys., Part 1
0021-4922,
28
(
9
), pp.
1728
1729
.
11.
Lichtenstein
,
A. I.
,
Katsnelson
,
M. I.
, and
Kotliar
,
G.
, 2001, “
Finite-Temperature Magnetism of Transition Metals: and LDA-DMFT Approach
,”
Phys. Rev. Lett.
0031-9007,
87
(
6
), pp.
067205
.
12.
,
M.
,
Moukara
,
M.
,
Majewski
,
J. A.
,
Vogl
,
P.
, and
Goerling
,
A.
, 1999, “
Exact Exchange Kohn–Sham Formalism Applied to Semiconductors
,”
Phys. Rev. B
0163-1829
59
(
15
), pp.
10031
10043
.
13.
Fernández
,
J. J.
,
Tablero
,
C.
, and
Wahnón
,
P.
, 2004, “
Application of the Exact Exchange Potential Method for Half Metallic Intermediate Band Alloy Semiconductor
,”
J. Chem. Phys.
0021-9606,
120
(
22
), pp.
10780
10785
.
14.
Palacios
,
P.
,
Wahnón
,
P.
,
Pizzinato
,
S.
, and
Conesa
,
J. C.
, 2006, “
Energetics of Formation of TiGa3As4 and TiGa3P4 Intermediate Band Materials
,”
J. Chem. Phys.
0021-9606,
124
,
014711
.
15.
Le Nagard
,
N.
,
Collin
,
G.
, and
Gorochov
,
O.
, 1979, “
Étude Structurale et Proprietés Physiques de CuCrS2
,”
Mater. Res. Bull.
0025-5408,
14
(
11
), pp.
1411
1417
.
16.
Le Nagard
,
N.
,
Gorochov
,
O.
, and
Collin
,
G.
, 1974, “
Structure Crystalline et Proprietés Physiques de CuxTiS2
,”
Mater. Res. Bull.
0025-5408,
10
(
12
), pp.
1287
1296
.